Andrey Tumarkin 1,* , Natalya Tyurnina 2, Zoya Tyurnina 2 , Nikolay Mukhin 3,4 , Olga Sinelshchikova 2, Alexander Gagarin 1, Sergey Sviridov 2, Andrey Drozdovsky 1, Eugeny Sapego 1 and Ivan Mylnikov 1
1 Department of Physical Electronics and Technology, Electrotechnical University, 5 prof. Popov Str., 197376 St. Petersburg, Russia; [email protected] (A.G.); [email protected] (A.D.); [email protected] (E.S.); [email protected] (I.M.) 2 Institute of Silicate Chemistry, Adm. Makarova emb., 2, 199155 St. Petersburg, Russia; [email protected] (N.T.); [email protected] (Z.T.); [email protected] (O.S.); [email protected] (S.S.) 3 Institute for Micro and Sensor Systems, Otto-von-Guericke-University Magdeburg, Universitätspl. 2, 39106 Magdeburg, Germany; [email protected] 4 Department of Engineering, University of Applied Sciences Brandenburg, Magdeburger Str. 50, 14770 Brandenburg an der Havel, Germany * Correspondence: [email protected]
Received: 10 November 2020; Accepted: 8 December 2020; Published: 10 December 2020
Abstract: Based on porous silicate glasses obtained by ion exchange, glass-ceramic materials containing a solid solution of barium-strontium titanate with a dielectric constant of more than 100 at microwaves, were synthesized for the ﬁrst time. Glass-ceramic structures were studied using X-ray diﬀraction, secondary electron microscopy, Mössbauer spectroscopy and porometry methods. Electrical characteristics such as permittivity and losses of as-prepared and annealed in oxygen medium samples were also investigated at microwaves. It was shown that the method of obtaining porous glasses, due to ion exchange between KFeSi glass and LiNO3 and NaNO3 melts, allows for controlling a wide range of pore sizes and makes it possible to form glass porous structures with pores of the required size. The eﬃciency of the process of ﬁlling a porous matrix with a ferroelectric ﬁller was investigated and the average depth of its penetration was estimated. It was shown that annealing glass-ceramic structures in an oxygen environment had a positive eﬀect on their structural and electrical characteristics. Glass-ceramic structures demonstrate a signiﬁcant increase in permittivity and a decrease in losses after high-temperature treatment in oxygen.
Keywords: glass-ceramic structures; barium-strontium titanate; ﬁlling of porous material; microwave
1. Introduction Ferroelectric (FE) materials are of great interest for microwave electronics because of their nonlinear response to an electric ﬁeld. On the basis of the ferroelectric materials, microwave devices such as tunable capacitors, delay lines, phase shifters, etc. [1–3] have been actively developed. However, like any functional materials, ferroelectrics have some disadvantages that limit their use in microwave devices. The weak points of FE materials are rather high microwave losses, a strong dependence of properties on temperature, and diﬃculties in matching a material with a large dielectric permittivity with microwave circuits [4,5]. One of the ways to minimize the above-mentioned disadvantages and improve the functional characteristics of FE materials is to create composite structures that combine ferroelectrics and linear dielectrics [6–9]. Composites containing lead titanate [6,7], barium and strontium titanates [8,9] have
Materials 2020, 13, 5639; doi:10.3390/ma13245639 www.mdpi.com/journal/materials Materials 2020, 13, 5639 2 of 15 been well studied. This approach allows to control the dielectric permittivity and losses by changing the concentration of ferroelectric inclusions in the composite. A distinctive feature of the approach is the uniform distribution of FE inclusions over the structure volume. Another approach to the formation of ferroelectric composite structures is the introduction of ferroelectric particles into the pore space of glass matrices [10,11]. This approach allows to adjust the size, shape, and relative location of ferroelectric inclusions by choosing the type of matrix. It also provides the possibility of obtaining structures with an artiﬁcially created spatial distribution of the dielectric permittivity. The advantage of this approach is the possibility of creating materials with new properties: structures with a purposefully formed dispersion characteristic; structures with a speciﬁed distribution of submillimeter-sized inhomogeneities, which determine their frequency and spatial selectivity when interacting with electromagnetic waves; structures with any speciﬁed permittivity with values from units to several hundred for the implementation of complex functional devices of microwave electronics, in which the matching of individual elements will be achieved due to a gradient change in the permittivity of the substrate. A promising way to create glass-ceramic structures for microwave applications is the introduction of barium-strontium titanate BaxSr1–xTiO3 (BST) into the pore space of a glass oxide matrix . By varying the component composition of the solid solution, the permittivity of the composite can be changed within a wide range . Oxide porous glasses exhibit thermal and chemical resistance, stable permittivity and low losses [14,15], which distinguishes them from other porous materials. To obtain porous glass materials the following methods are used: through chemical etching (leaching) of two-phase glass with interpenetrating phases , the sol-gel method , template synthesis method  and replica method , which consists in sequential mixing of glass powder, solution for impregnation of the polymer matrix with further high temperature treatment of the ﬁnished mixture. The disadvantages of these methods are rather strict limitations on the pore size. An alternative to the above approaches is a method for producing silicate glasses with a porous structure due to ion exchange between alkaline glass cations and salt melt cations , which allows one to control the size of pores in a wide range. The advantage of this method is the possibility of obtaining new porous glass materials with the required distribution of properties by volume, depending on the composition of the glass and the salt melt, the ionic radii of the exchanging cations, and the temperature and time of interaction. The aim of this paper is to study the possibilities of creating glass-ceramic ferroelectric structures based on barium-strontium titanate, introduced in the pore space of silicate glass, formed by ion exchange between alkaline glass cations and salt melt, and to characterize their structure and electrical properties at microwaves.
2. Materials and Methods
2.1. Materials Synthesis and Characterization
The synthesis of potassium-iron-silicate glass (KFeSi glass) of the composition 15K2O-20Fe2O3- 65SiO2, mol.% was carried out from chemically pure reagents-K2CO3, FeO, Fe2O3 and SiO2 in a platinum crucible at a temperature of 1450 ◦C for 2 h, followed by annealing at a temperature of 550 ◦C. Glass samples were quenched in air by casting the melt on a steel mold. In order to form porous glasses, ion exchange processing of model glass plates was performed in NaNO3 and LiNO3 melts at temperatures of 450 ◦C with isothermal exposure for 9 h. The duration of isothermal treatment was chosen in such a way as to provide thorough processing of the glass plate, taking into account the data obtained earlier . Since K+ ions are replaced by Li+ and Na+ due to ion exchange, the glass processed in LiNO3 and in NaNO3 will be designated as Li2O-Fe2O3-SiO2 (LiFeSi) and as Na2O-Fe2O3-SiO2 (NaFeSi), respectively. The geometric parameters of the porous structure of glass after ion exchange and subsequent removal of the salt melt by treatment in water were determined by reference porometry of glass samples Materials 2020, 13, 5639 3 of 15 in the form of a disk with a diameter of 23 mm and a thickness of 2 mm, at the Porotech 3.1 installation in the resource center of St. Petersburg state University “Thermogravimetric and calorimetric research methods”. Electronic micrographs of the studied glass samples were obtained using a Zeiss SUPRA 40VP scanning electron microscope (Carl Zeiss, Munich, Germany) with an SE2 detector (SEM) in the resource center of St. Petersburg state University “Nanotechnologies”. X-ray diﬀraction images (XRD) of samples were obtained using a DRON-3 diﬀractometer (radiation wavelength 0.154 nm, Cu Kα) (Burevestnik, St. Petersburg, Russia) at room temperature. The degree of iron oxidation in the glasses was determined by Mössbauer spectroscopy (nuclear gamma resonance) on the MC-1107 Em spectrometer (Institute for Analytical Instrumentation RAS, St. Petersburg, Russia). The samples were measured in the transmission mode with constant acceleration, using 57Co in the rhodium matrix as the source. The registered spectra were processed using a specialized MossFit software package. In order to synthesis barium-strontium titanate (BST), the initial mixtures were prepared from hydrated titanium dioxide, which was obtained by the interaction between TiCl4 and dilute ammonia NH4OH at a reaction medium pH equal to 9.5. The residue was washed of impurities, and then dissolved in 1.4 mol/L solution of nitric acid. The solution of TiO(NO3)2 was obtained. The gravimetric method was used to control the concentration of TiO2 in the obtained solution of titanyl nitrate. It equaled 0.1 g/mL. Aqueous solutions of Ba(NO3)2 or Ba(CH3COO)2 and Sr(NO3)2 were introduced into the obtained solution of titanyl nitrate according to the stoichiometry of the forming complex oxide. Glycine (Vekton, St. Petersburg, Russia) was also added. The solutions containing amount of strontium nitrate were obtained corresponding to the calculated stoichiometry of Ba0.7Sr0.3TiO3. After the evaporation of excess water, porous glasses were placed in the sol and were kept in it at 80 ◦C within 2 h. After impregnation, the glass was heat treated at 500 ◦C within 3 h in air during which crystallization of barium-strontium titanate occurred with a low content of impurity phases both on the glass surface and in its pore space. The procedure of soaking a glass sample in the sol, followed by heat treatment, was repeated 2 times. After preparing glass samples with BST in a porous space, some of them were annealed in an oxygen stream at 500 ◦C for 2 h in order to increase the crystallinity of barium-strontium titanate.
2.2. Electrical Characterization The dielectric (ε) permittivity of samples, as well as dependencies ε on frequency in microwaves were estimated by the Nicholson–Ross method . For this purpose, a microstrip transmission line connected to the vector network analyzer was used. In this study the frequency dependences of the modulus of the reflection coefficient and the phase of the transmission coefficient were measured in the frequency range of 3–10 GHz, when samples were superimposed on the transmission line. Then, these measurement data were recalculated into dielectric permittivity. Dielectric losses (tan δ) of ceramic-glass structures were measured in plane-parallel samples with silver paste electrodes at a frequency of 1 MHz and room temperature by Agilent E4980A LCR meter (Agilent, Santa Clara, CA, USA).
3. Results and Discussion
3.1. Structural and Morphologic Characterization of Porous Glasses
Ion exchange treatment of 15K2O-20Fe2O3-65SiO2 glass in a LiNO3 and NaNO3 melt at a temperature below the glass transition temperature (Tg) leads to the formation of a porous structure in glass , as schematically shown in Figure1 using the example of a KFS and NaNO 3 interaction. In another study , it was established that the kinetics and nature of the interaction of glasses with molten salts substantially depend on the direction of the ﬂuxes of exchanging cations. With the same ion exchange treatment, in the case where the ﬂow of a cation with a smaller ionic radius is directed from the molten salt to glass, the interaction process leads to the formation of an opaque diﬀusion zone, the length of which is many times larger than the size of the zone during ion exchange with the Materials 2020, 13, 5639 4 of 15 opposite direction of alkaline cation ﬂuxes. The reason for the observed anomalies of the ion exchange process is that atMaterials temperatures 2020, 13, x FOR PEER below REVIEW the glass transition temperature silicon-oxygen4 of 16 groups cannot change their orientationchange their andorientation position and position in space. in space. Replacing Replacing the the alkaline alkaline glass cations glass with cations cations with with cations with a smaller ionic radiusa smaller and, ionic accordingly,radius and, accordingly, with awith higher a higher ﬁeld field strength strength leads leads to tensile to stresses tensile at T stresses < Tg. at T < Tg.
Figure 1. IonFigure exchange 1. Ion exchange process process between between KFeSi KFeSi glassglass and NaNO and3 melt. NaNO 3 melt.
Figure 2 shows diffractograms of annealed and tempered KFeSi glass, as well as glasses Figure2 showssubjected di toﬀ ractogramsion exchange treatment of annealed in LiNO3 andand NaNO tempered3 melts. XRD KFeSi analysis glass, data asindicate well that as ion glasses subjected to ion exchangeexchange treatment in NaNO in3 LiNO and LiNO3 and3 melts NaNO has different3 melts. effects XRD on the analysis formation of data crystal indicate phases in thatthe ion exchange samples under study. Figure 2 indicates the presence of crystalline iron oxide, presumably γ-Fe2O3, in NaNO3 andboth LiNO in the3 meltsinitial glass has (curves diﬀ erent1 and 2) eandﬀects in the on porous the glass formation after ion exchange of crystal (curves phases three and in the samples under study. Figurefour). 2The indicates ion exchange the procedure, presence which of takes crystalline place at a irontemperature oxide, of presumably450 °C for 9 h, leadsγ-Fe to a2 O3, both in the initial glass (curveschange 1 in and the 2)phase and composition in the porous and crystal glass structure after of ion iron exchange oxide: for both (curves porous threeglasses, and the four). The ion intensity of reflexes decreases for most phases, for LiFeSi glass a rather intense peak (320) appears. exchange procedure,Comparison which of curves takes two and place three atallows a temperature us to suggest thatof ion450 exchange◦C forin the 9 NaNO h, leads3 melt leads to a change in the phase compositionto a decrease and crystal in the content structure of the crystalline of iron phase oxide: of iron for oxide both in the porous NaFeSi glasses,glass. On the the contrary, intensity of reﬂexes the presence of rather intense reflexes (311), (320), and (440) in LiFeSi porous glass indicates a decreases for mostredistribution phases, of forthe crystalline LiFeSi glassphases of a iron rather oxide intense as a result peakof ion exchange (320) appears. (comparison Comparison of curves of curves two and four). In addition to γ-Fe2O3, the X-ray image of LiFeSi glass shows reflexes indicating the two and three allows us to suggest that ion exchange in the NaNO3 melt leads to a decrease in the presence of the Li5FeO4 phase. content of the crystalline phase of iron oxide in the NaFeSi glass. On the contrary, the presence of rather intense reﬂexes (311), (320), and (440) in LiFeSi porous glass indicates a redistribution of the crystalline phases of iron oxide as a result of ion exchange (comparison of curves two and four). In addition to
γ-Fe2O3, the X-rayMaterials image 2020, 13, x ofFOR LiFeSi PEER REVIEW glass shows reﬂexes indicating the presence of5 theof 16 Li5FeO4 phase.
● - γ - Fe2O3 [24-81] ▪ - Li5FeO4 [24-624] (1 1 1) 1 (1 (2 0 1) 0 (2 (2 1 1) 1 (2 (0 0 1) 0 (0 (4 0 0) 0 (4 (2 2 0) 2 (2 (3 2 0) 2 (3 (3 1 1) 1 (3 (4 4 0) (4 4 (5 1 1) 1 (5 (1 1 2) 1 (1 4
10 15 20 25 30 35 40 45 50 55 60 65 70 2θ, deg
Figure 2. X-rayFigure di 2.ﬀ X-rayraction diffraction images images (XRD) (XRD) patterns patterns of KFS of glass KFS samples: glass 1—tempered samples: glass; 1—tempered 2— glass; annealed glass; 3—glass after the ion exchange treatment in NaNO3 melt at 450 °С for 9 h; 4—glass 2—annealed glass; 3—glass after the ion exchange treatmentγ in NaNO3 melt at 450 ◦C for 9 h; after the ion exchange treatment in LiNO3 melt at 450 °С for 9 h (●— -Fe2O3, —Li5FeO4). 4—glass after the ion exchange treatment in LiNO3 melt at 450 ◦C for 9 h ( —γ-Fe2O3 Pdf No 24-81 , γ • —Li5FeO4 PdfIt is No known 24-624 that [magnetite24]). (Fe3O4) and maghemite ( -Fe2O3) cannot be distinguished by the X- ray method, because both oxides have a spinel-type structure. To identify the phases of iron oxides in the studied glasses, the Mössbauer spectroscopy method was used, since the parameters of the hyperfine interaction of the Mössbauer spectra of magnetite and maghemite differ significantly. Figures 3 and 4 show the Mössbauer spectra of NaFeSi and LiFeSi glasses, respectively. Table 1 below shows hyperfine parameters: isomeric (or chemical) shift (IS), quadrupole splitting (QS), and line widths at half height (G). It can be seen from the presented data, that the spectra of the studied glasses are a superposition of two quadrupole doublets. The values of the isomeric shift suggest that all iron atoms are in the +3 valence state in unsymmetrical surroundings in both NaFeSi and LiFeSi glasses.
Materials 2020, 13, 5639 5 of 15
It is known that magnetite (Fe3O4) and maghemite (γ-Fe2O3) cannot be distinguished by the X-ray method, because both oxides have a spinel-type structure. To identify the phases of iron oxides in the studied glasses, the Mössbauer spectroscopy method was used, since the parameters of the hyperﬁne interaction of the Mössbauer spectra of magnetite and maghemite diﬀer signiﬁcantly. Figures3 and4 show the Mössbauer spectra of NaFeSi and LiFeSi glasses, respectively. Table1 below shows hyperﬁne parameters: isomeric (or chemical) shift (IS), quadrupole splitting (QS), and line widths at half height (G). It can be seen from the presented data, that the spectra of the studied glasses are a superposition of two quadrupole doublets. The values of the isomeric shift suggest that all iron atoms are in the +3 valence state in unsymmetrical surroundings in both NaFeSi and LiFeSi glasses. Materials 2020, 13, x FOR PEER REVIEW 6 of 16
Transmission, a.u. Transmission, a.u.
FigureFigure 3. Mössbauer 3. Mössbauer spectrum spectrum of of the the NaFeSi NaFeSi sample sample obtained obtained at room temperature at room temperature and in an external and in an external magneticmagnetic ﬁeld. field. Transmission, a.u. Transmission, a.u.
Figure 4. Mössbauer spectrum of the LiFeSi sample obtained at room temperature and in an external Figure 4. Mössbauer spectrum of the LiFeSi sample obtained at room temperature and in an external magneticmagnetic ﬁeld. field.
Table 1. Hyperfine parameters obtained from Mössbauer spectrum of the NaFeSi and LiFeSi samples.
Sample # G (mm/s) IS (mm/s) QS (mm/s) % 1 0.514 ± 0.025 0.249 ± 0.004 1.163 ± 0.040 64.00 NaFeSi 2 0.351 ± 0.031 0.232 ± 0.004 0.714 ± 0.024 36.00 1 0.550 ± 0.024 0.266 ± 0.003 1.242 ± 0.036 55.88 LiFeSi 2 0.453 ± 0.026 0.254 ± 0.003 0.753 ± 0.027 44.12
Materials 2020, 13, 5639 6 of 15
Table 1. Hyperﬁne parameters obtained from Mössbauer spectrum of the NaFeSi and LiFeSi samples.
Sample # G (mm/s) IS (mm/s) QS (mm/s) % 1 0.514 0.025 0.249 0.004 1.163 0.040 64.00 NaFeSi ± ± ± 2 0.351 0.031 0.232 0.004 0.714 0.024 36.00 ± ± ± 1 0.550 0.024 0.266 0.003 1.242 0.036 55.88 LiFeSi ± ± ± 2 0.453 0.026 0.254 0.003 0.753 0.027 44.12 Materials 2020, 13, x FOR PEER REVIEW ± ± ± 7 of 16
As shown in another study [,25], the Fe33++ cationscations appear appear to to be be in in tetrahedral surroundings. surroundings. SufficientlySuﬃciently large values of quadrupole splitting indicate a significant signiﬁcant distortion of polyhedra in the glass structure. It follows that iron Fe++33 isis present present in in the the studied studied glasses glasses both both as as part part of of the the crystalline oxide γ-Fe-Fe22OO3 3andand directly directly in in the the glass glass structure. structure. The difference diﬀerence between the spectra lies in the shapeshape of the doublets:doublets: in the case of the NaFeSi sample, the doublet has a more symmetrical shape th thanan for LiFeSi, which indicates a more crystalline structure of the latter. Figure5 5 showsshows datadata onon pore sizes in NaFeSi and LiFeSi glasses obtained by by reference reference porometry. porometry. Analysis of porometric data shows that at an ion exchange temperature of 450 °◦СC,, 14% of the pores in the the NaFeSi NaFeSi glass glass have have a a size size in in the the range range of of 1–100 1–100 nm, nm, and and 57% 57% in inthe the range range of of1–10 1–10 microns; microns; in LiFeSiin LiFeSi glass, glass, the thecontent content of pores of pores with with a size a sizein the in range the range of 1–10 of 1–10 nm is nm 35%, is 35%,and in and the in range the range of 1–10 of 1–10microns—49%. microns—49%. The porosity The porosity values values of these of theseglasses glasses by weight by weight are 0.033 are 0.033cm3/g cmfor3 /NaFeSig for NaFeSi and 0.041 and cm0.0413/g cmfor3 /LiFeSi,g for LiFeSi, with a with specific a speciﬁc surface surface area of area 3.07 of m 3.072/g and m2/ g5.0 and m2 5.0/g, respectively. m2/g, respectively.
60 57 49 50
Yield, % 20 14 10 6 10 4
0 NaNO3, 450 °C, 9 h. LiNO3, 450 °C, 9 h.
1-100 nm 100 nm-1 mkm 1-10 mkm 10-30 mkm
Figure 5.5. TheThe distributiondistribution of of the the pore pore sizes sizes for for glasses glasses after after the ionthe exchange ion exchange in NaNO in NaNO3 and LiNO3 and3 LiNOmelts.3 melts. 3.2. Characterization of BST in Porous Space of Glass 3.2. CharacterizationMicrographs of of theBST surface in Porous of Space the original of Glass KFeSi glass (a), LiFeSi (b) and NaFeSi (c) glasses obtainedMicrographs as a result of ofthe ion surface exchange, of the as welloriginal as NaFeSi KFeSi glass (d)(a), withLiFeSi embedded (b) and NaFeSi barium-strontium (c) glasses obtainedtitanate are as showna result in of Figure ion exchange,6. According as well to SEM as NaFeSi analysis glass data, (d) the with morphology embedded of barium-strontium the glass surface titanateafter ion are exchange shown in treatment Figure 6. is According in good agreement to SEM analysis with thedata, data the of morphology standard reference of the glass porometry. surface Theafter micrographs ion exchange allow treatment us to estimate is in good changes agreement in the surface with the morphology data of standard of the original reference glass porometry. as a result Theof ion micrographs exchange in allow NaNO us3 toand estimate LiNO3 meltschanges and in as th ae resultsurface of morphology the introduction of the of original barium-strontium glass as a resulttitanate of into ion theexchange pore space in NaNO of the3 glass and matrix.LiNO3 melts SEM dataand indicateas a result that of the the ion introduction exchange of of potassium barium- withstrontium lithium titanate and with into natrium the pore changes space of the the surface glass of matrix. the original SEM data glass indicate in diﬀerent that ways the ion (see exchange Figure6b,c). of potassiumCrystal structures with lithium that can and be with attributed natrium to changes the orthorhombic the surface phase of the of original Li5FeO glass4 are in clearly different visible ways on (see Figure 6b,c). Crystal structures that can be attributed to the orthorhombic phase of Li5FeO4 are clearly visible on the surface of LiFeSi glass. The micrograph of NaFeSi glass shows the presence of a fine-grained structure formed as a result of ion exchange. Based on the porometric data and the results of electron microscopy, it can be assumed that the glass subjected to ion exchange in the LiNO3 melt shows a more developed porous structure, which can have a positive effect on the efficiency of introducing barium-strontium titanate into it. Figure 6d indicates that the impregnation of porous glasses with BST sol leads to uniform pore filling and the formation of a surface without significant cavities.
Materials 2020, 13, 5639 7 of 15
the surface of LiFeSi glass. The micrograph of NaFeSi glass shows the presence of a ﬁne-grained structure formed as a result of ion exchange. Based on the porometric data and the results of electron microscopy, it can be assumed that the glass subjected to ion exchange in the LiNO3 melt shows a more developed porous structure, which can have a positive eﬀect on the eﬃciency of introducing barium-strontium titanate into it. Figure6d indicates that the impregnation of porous glasses with BST sol leads to uniform pore ﬁlling and the formation of a surface without signiﬁcant cavities. Materials 2020, 13, x FOR PEER REVIEW 8 of 16
217 FigureFigure 6. 6. SEM-imageSEM-image of ofthe the surface surface of the of theoriginal original KFeSi KFeSi (a); LiFeSi (a); LiFeSi glass glassobtained obtained as a result as a of result ion
218 exchangeof ion exchange in LiNO in3 (b LiNO); NaFeSi3 (b );glass NaFeSi obtained glass as obtained a result of as ion a resultexchange of ion in NaNO exchange3 (c); inNaFeSi-based NaNO3 (c); 219 compositeNaFeSi-based containing composite BaSrTiO containing3 (d). BaSrTiO3 (d).
220 FigureFigure 7 shows didiffractogramsﬀractograms of of NaFeSi/BST NaFeSi/BST an andd LiFeSi/BST LiFeSi/BST glass-ceramic glass-ceramic samples samples before before and and 221 afterafter annealing annealing in in an an oxygen oxygen atmosphere. atmosphere. Since Since the the matrix matrix glass glass is an is X-ray an X-ray amorphous amorphous material, material, the 222 low-intensitythe low-intensity peaks peaks from frombarium-strontium barium-strontium titanate titanate in the X-ray in the diffraction X-ray diﬀraction pattern patternare due areto the due fact to 223 thatthe factthe pore that thevolume pore is volume not completely is not completely filled with ﬁlled the crystalline with the crystalline phase, which phase, is a which typical is situation a typical 224 forsituation porous for structures. porous structures.From the XRD From analysis the XRDdata, analysisit follows data, that high-temperature it follows that high-temperature treatment in an 225 oxygentreatment atmosphere in an oxygen has atmospherea positive effect has a on positive the crystal eﬀect structure on the crystal of barium-strontium structure of barium-strontium titanate—the 226 diffractogramstitanate—the di ofﬀractograms samples after of annealing samples after clearly annealing show the clearly increase show in the intensity increase of in(111) intensity reflexes. of This (111) 227 allowsreﬂexes. us Thisto expect allows an us improvement to expect an in improvement the dielectric in characteristics the dielectric of characteristics glass-ceramic of structures glass-ceramic as a 228 resultstructures of annealing—the as a result of increase annealing—the in the dielectric increase constant in the dielectric and reduction constant in losses. and reduction In addition in to losses. BST 229 peaks,In addition the XRD to BST images peaks, of the glasses XRD imagesboth before of glasses and bothafter beforeannealing and show after annealingreflexes indicating show reﬂexes the 230 presenceindicating of the the presence γ-Fe2O3 phase of the (markedγ-Fe O asphase ∗) with (marked an almost as ) unchanged with an almost intensity. unchanged intensity. 2 3 ∗ 231 Attention is drawn to the appearance of the more pronounced and intensive reflexes at the 232 angles of 47 ° and 48 ° on the diffractograms of samples subjected to high-temperature processing 233 (indicated as +) which may be due to the presence of crystal phases of secondary barium polytitanate 234 in the composite, presumably BaTi4O9. The increase in polytitanate reflex intensity can be explained 235 by the partial conversion of barium titanate to polytitanates in an oxygen medium . Barium 236 polytitanates, such as BaTi2O5, BaTi3O7, BaTi4O9 and so on, are intermediate products that can be 237 formed in a stoichiometric mixture of reagents, depending on the temperature conditions of the 238 synthesis process. Many of polytitanates have a crystal structure similar to BaTiO3, which makes it 239 difficult to identify them by XRD. Generally being linear dielectrics with a permittivity scale of 10– 240 40, these compounds have a greater influence on the final electrical properties of the composite, the 241 greater their content in it .
Materials 2020, 13, 5639 8 of 15 Materials 2020, 13, x FOR PEER REVIEW 9 of 16 + (002)+ +(260) NaFeSi/BST BST(211) BST(210) * (311) BST(200) BST(111) BST(110)
30 35 40 45 50 55 60 2θ, deg
Figure 7. XRD of BaSrTiO3 in porous glass matrices before and after annealing in oxygen atmosphere Figure( —γ -Fe7. XRDO Pdfof BaSrTiO No 24-813 in [24 porous]; +—presumably glass matrices BaTi beforeO Pdfand Noafter 34-70 annealing ). in oxygen atmosphere ∗ 2 3 4 9 (∗—γ-Fe2O3 Pdf No 24-81 ; +—presumably BaTi4O9 Pdf No 34-70 ). Attention is drawn to the appearance of the more pronounced and intensive reﬂexes at the angles 3.3.of Electrical 47◦ and 48 Characterization◦ on the diﬀractograms of BST-Glass of samples Structures subjected to high-temperature processing (indicated as +) which may be due to the presence of crystal phases of secondary barium polytitanate in the composite, The frequency dependences of the permittivity of the base KFeSi glass, as well as NaFeSi/BST presumably BaTi4O9. The increase in polytitanate reﬂex intensity can be explained by the partial and LiFeSi/BST glass-ceramic samples before and after annealing in an oxygen environment are conversion of barium titanate to polytitanates in an oxygen medium . Barium polytitanates, such as shown in Figure 8. It can be seen from the presented data that in the studied frequency range, the BaTi2O5, BaTi3O7, BaTi4O9 and so on, are intermediate products that can be formed in a stoichiometric permittivity of both NaFeSi/BST and LiFeSi/BST samples weakly depends on the frequency. The mixture of reagents, depending on the temperature conditions of the synthesis process. Many of NaFeSi/BST structure shows a permittivity of about 40, which increases slightly after annealing. The polytitanates have a crystal structure similar to BaTiO3, which makes it diﬃcult to identify them by LiFeSi/BST one exhibits a significantly higher permittivity and shows an almost two-fold increase in XRD. Generally being linear dielectrics with a permittivity scale of 10–40, these compounds have a it as a result of annealing. The increase in the permittivity is obviously related to the improvement in greater inﬂuence on the ﬁnal electrical properties of the composite, the greater their content in it . the crystal structure of the barium-strontium titanate as a result of annealing in an oxygen atmosphere3.3. Electrical [28,29]. Characterization The decrease of BST-Glassin dielectric Structures permittivity under the applied DC voltage was about 1% under electric field strength of 10 V/cm. The frequency dependences of the permittivity of the base KFeSi glass, as well as NaFeSi/BST and The decrease in tan δ of the glass-ceramic samples after their high-temperature treatment in O2 LiFeSi/BST glass-ceramic samples before and after annealing in an oxygen environment are shown in is shown in the insert of Figure 8. One of the possible explanations for this improvement in dielectric Figure8. It can be seen from the presented data that in the studied frequency range, the permittivity of losses both for NaFeSi/BST and for LiFeSi/BST structures may be due to a decrease in the number of both NaFeSi/BST and LiFeSi/BST samples weakly depends on the frequency. The NaFeSi/BST structure oxygen vacancies in the perovskite lattice of BST. It is known that barium-strontium titanate is often shows a permittivity of about 40, which increases slightly after annealing. The LiFeSi/BST one exhibits deficient in oxygen, i.e., there are vacancies in the oxygen sublattice . When located near oxygen a signiﬁcantly higher permittivity and shows an almost two-fold increase in it as a result of annealing. vacancies, titanium ions Ti4+ can capture free electrons and turn into Ti3+. The presence of Ti3+ ions in The increase in the permittivity is obviously related to the improvement in the crystal structure of the the lattice leads to the appearance of “hopping” conductivity, when electrons can move between barium-strontium titanate as a result of annealing in an oxygen atmosphere [28,29]. The decrease in different Ti3+ titanium ions and increase dielectric losses. It is obvious that annealing in an oxygen dielectric permittivity under the applied DC voltage was about 1% under electric field strength of 10 V/cm. atmosphere restores the missing oxygen in the crystal lattice and, as a result, reduces losses by two to three times. A change in the charge state of iron ions (as a result of oxidation from Fe3+ to Fe4+) may be another possible reason for the change in losses due to high-temperature treatment of iron- containing samples in oxygen [31–33].
Materials 2020, 13, 5639 9 of 15 Materials 2020, 13, x FOR PEER REVIEW 10 of 16
FigureFigure 8.8. DielectricDielectric permittivitypermittivity ofof KFeSiKFeSi basebase glass,glass, andandNaFeSi NaFeSi/BST/BSTand andLiFeSi LiFeSi/BST/BSTglass-ceramic glass-ceramic samples.samples. TheThe insertinsert presentspresents dielectricdielectric losseslosses ofof NaFeSiNaFeSi/BST/BST andand LiFeSiLiFeSi/BST/BST glass-ceramicglass-ceramic samplessamples beforebefore andand afterafter annealingannealing in in an an oxygen oxygen atmosphere. atmosphere.
3.4. PorousThe decrease Matrix inFilling tan δ Estimationof the glass-ceramic samples after their high-temperature treatment in O2 is shown in the insert of Figure8. One of the possible explanations for this improvement in dielectric lossesUnder both for various NaFeSi technological/BST and for regimes LiFeSi/BST of forming structures a composite may be due system, to a decrease the ferroelectric in the number filler can of oxygenimpregnate vacancies a part in of the theperovskite porous matrix, lattice leaving of BST. some It is inner known pore that layers barium-strontium free. In this case, titanate the dielectric is often deﬁcientconstant inof oxygen,the composite i.e., there structure are vacancies turns inout the to oxygenbe lower sublattice than expected. . When In order located to nearestimate oxygen the vacancies,average penetration titanium ions depth Ti4 +(hcan) of capturea ferroelectric free electrons filler into and a turnporous into matrix Ti3+. Thewith presence the H thickness, of Ti3+ ions the infollowing the lattice analytical leads to models the appearance can be used. of “hopping” conductivity, when electrons can move between diﬀerentFigure Ti3 +9atitanium schematically ions and shows increase a dielectrictypical case. losses. The It iscomposite obvious thatsample annealing in general in an oxygencan be atmosphereconditionally restores divided the into missing several oxygen layers. in the Near-surface crystal lattice layers and, as(L1 a) result,are a reducesferroelectric-filled losses by two glass to threematrix, times. since A changethe pore in thefilling charge process state ofoccurs iron ionson both (as a resultsides. ofThe oxidation central fromlayer Fe (3L2+ )to of Fe the4+) mayporous be anotherstructure possible can bereason left empty for the if changethe technological in losses due process to high-temperature of pore filling is treatment not optimal, of iron-containing and between samplesthese layers, in oxygen there [are31– intermediate33]. layers (IL), in which some parts of the pores are occupied by the ferroelectric phase, and the other parts of the pores remains empty. This multilayer model is the most 3.4.common Porous case Matrix for Fillingthe technology Estimation used in this study. Several simpler situations are shown in Figure 9b–e: only porous matrix (Figure 9b); all pores are filled with ferroelectric (Figure 9c); a model, when Under various technological regimes of forming a composite system, the ferroelectric ﬁller can the intermediate layer can be neglected (Figure 9d); a model, where the central layer is particularly impregnate a part of the porous matrix, leaving some inner pore layers free. In this case, the dielectric filled (Figure 9e). Electrodes are located above and below the composite film, forming a capacitor. constant of the composite structure turns out to be lower than expected. In order to estimate the average penetration depth (h) of a ferroelectric ﬁller into a porous matrix with the H thickness, the following analytical models can be used. Figure9a schematically shows a typical case. The composite sample in general can be conditionally divided into several layers. Near-surface layers (L1) are a ferroelectric-ﬁlled glass matrix, since the pore ﬁlling process occurs on both sides. The central layer (L2) of the porous structure can be left empty if
Materials 2020, 13, 5639 10 of 15 the technological process of pore ﬁlling is not optimal, and between these layers, there are intermediate layers (IL), in which some parts of the pores are occupied by the ferroelectric phase, and the other parts of the pores remains empty. This multilayer model is the most common case for the technology used in this study. Several simpler situations are shown in Figure9b–e: only porous matrix (Figure9b); all pores are ﬁlled with ferroelectric (Figure9c); a model, when the intermediate layer can be neglected
(FigureMaterials9d); 2020 a, model,13, x FOR where PEER REVIEW the central layer is particularly ﬁlled (Figure9e). Electrodes are located11 of 16 above and below the composite ﬁlm, forming a capacitor.
Figure 9. The composite ﬁlm model (a) and its simpliﬁed particular cases: only porous matrix (b); Figure 9. The composite film model (a) and its simplified particular cases: only porous matrix (b); all all pores are ﬁlled (c); a model where the intermediate layer can be neglected (d); a model where the pores are filled (c); a model where the intermediate layer can be neglected (d); a model where the central layer is particularly ﬁlled (e), where 1 is ferroelectric, 2 is air, m is medium matrix. central layer is particularly filled (e), where 1 is ferroelectric, 2 is air, m is medium matrix. For the two-phase air/glass (Figure9b) and ferroelectric /glass (Figure9c) systems, the e ﬀective For the two-phase air/glass (Figure 9b) and ferroelectric/glass (Figure 9c) systems, the effective dielectric constant (εjm) can be calculated in diﬀerent ways if the volume fraction of the dispersed dielectric constant (εjm) can be calculated in different ways if the volume fraction of the dispersed phase (ϕ) and the dielectric constants of the dispersed phase (εj) and medium matrix (εm) are known. phase (φ) and the dielectric constants of the dispersed phase (εj) and medium matrix (εm) are known. Various models are used for estimating the eﬀective dielectric constant. Diﬀerent models have to be Various models are used for estimating the effective dielectric constant. Different models have to be used to correctly describe the eﬀects under consideration, since the eﬀective dielectric properties of the used to correctly describe the effects under consideration, since the effective dielectric properties of composite depend on the peculiarities of phase mixing and the nature of their interaction, the ﬁller the composite depend on the peculiarities of phase mixing and the nature of their interaction, the concentration, its morphology, and the microstructure of the composite. Many of the above aspects filler concentration, its morphology, and the microstructure of the composite. Many of the above depend on the technological conditions for obtaining the composite [34–37]. aspects depend on the technological conditions for obtaining the composite [33–36]. The simplest mixing model gives : The simplest mixing model gives : εn (ω) = εn (ω)(ϕ 1) + εn(ω)ϕ, (1) jm nn()m () − j n() ε ωω= εφ−()1+εφ ω, (1) jm m j where ω is the frequency; n is the empirical parameter and ranges from 1 to 1, depending on composite − morphology.where ω is Forthe nfrequency;equal to one, n is this the is empirical the model parameter of an ideal and mechanical ranges mixturefrom −1 [to38 ].1, The depending deviation on ofcompositen from unity morphology. corresponds For ton equal the deviation to one, this of is the the mixture model of from an ideal the ideal mechanical case. Inmixture practice, .n Theis determineddeviation of from n from the unity experiment, corresponds by approximating to the deviation the of experimental the mixture from data bythe Equation ideal case. (1), In forpractice, this reasonn is determinedn is called thefrom empirical the experiment, parameter. by approximat For the modeling the in Figure experimental9, the index data jby is oneEquation or two (1), for for ferroelectric-this reason n or is air-ﬁlled called the (i.e., empirical pores) glass,parameter. respectively. For the model in Figure 9, the index j is one or two for ferroelectric-Another model or air-filled of thedielectric (i.e., pores) constant glass, ofrespectively. a two-phase system is represented by the equation : Another model of the dielectric constant of a two-phase system is represented by the equation : kϕ εm(ω) ε (ω) − j εjm = εj(ω)1 + , (2) (1 ϕ) εm(kωφε()) ε() ωj(ω− ε) ()+ ωkεm(ω) ()−+ mj− ε = ε ω 1, (2) jm j ()1−−+φε()() ω εω ()k ε() ω mj m
where k can vary greatly and relates to the filler microstructure [38–40]. When k is equal to three, it gives a Maxwell–Garnett equation , which is a model based on the analysis of the average field values for a single spherical inclusion in a continuous medium of a polymer matrix. In another study , it was established that the composite sample was satisfactorily described with k equal to 20. The Bruggeman model gives the following equation :
Materials 2020, 13, 5639 11 of 15 where k can vary greatly and relates to the ﬁller microstructure [39–41]. When k is equal to three, it gives a Maxwell–Garnett equation , which is a model based on the analysis of the average ﬁeld values for a single spherical inclusion in a continuous medium of a polymer matrix. In another study , it was established that the composite sample was satisfactorily described with k equal to 20. The Bruggeman model gives the following equation :
εm(ω) εjm(ω) εj(ω) εjm(ω) (1 ϕ) − + ϕ − = 0. (3) − εm(ω) + 2εjm(ω) εj(ω) + 2εjm(ω)
This model is based on the mean ﬁeld theory and considers the composite in the form of repeating elements consisting of a matrix phase containing the inclusion of a spherical ﬁller in the center. The eﬀective dielectric constant εeﬀ of the complete three-phase system of the multilayer model (Figure9a) is determined by the dielectric properties of each of the layers and their thicknesses, according to Equation (4):
H 2h ∆h 4∆h H 2h ∆h = − + + − − , (4) εeﬀ(ω) ε1m(ω) ε1m(ω) + ε2m(ω) ε2m(ω) where indices one, two and m refer to the ferroelectric phase, air and matrix medium, respectively; ε1m and ε2m are the eﬀective dielectric constant of the ferroelectric/matrix and porous matrix, respectively; ω is the circular frequency; H, h, ∆h are the thickness of the composite ﬁlm, the average penetration depth of ferroelectric ﬁller and the thickness of the intermediate layers, respectively. Equation (4) was derived from geometric considerations based on the sequence of layer arrangements shown in Figure9a. For this model the values of ε1m and ε2m can be calculated according to one of the Equations (1)–(3), for which the volume fraction of the dispersed phase will be the same and equal to the volume fraction of pores in the glass matrix. The thickness of the intermediate layer can be estimated from considerations of the average statistical ﬂuctuation theory  and diﬀusion limitation of the process  of introducing a ferroelectric ﬁller into a porous matrix, according to Equation (5): p ∆h = h/ √N, N ϕN D τ/H, (5) ≈ 1 1 where N is the number of ﬁller microstructural particles involved in the process; N1 and D1 are the total number and diﬀusion coeﬃcient of the ﬁller particles; τ is the processing time. Solving the system of the equations above, it is possible to estimate the process eﬃciency of the composite formation, determining how deeply the ferroelectric ﬁller was introduced into the porous matrix. Equation (4) can be simpliﬁed by replacing the three-phase system of the general multilayer model (Figure9a) with the special ones shown in Figure9d,e:
H 2h H 2h H 4h H 4(H 2h) = + − ; = − + − , (6) εeﬀ(ω) ε1m(ω) ε2m(ω) εeﬀ(ω) ε1m(ω) ε1m(ω) + ε2m(ω) where the left equation corresponds to the case of a series layer model of completely ﬁlled and empty pores, and the right equation corresponds to the case of a half-ﬁlled central layer. By solving Equation (4) or (6), as well as substituting one of Equations (1)–(3) in them, depending on the choice of the model, it is possible to estimate the penetration depth (h). For the series layer model (Figure9d) the penetration depth using Equation (1) can be estimated as: εn (ω)(ϕ ) + εn(ω)ϕ εn (ω)(ϕ ) + εn(ω)ϕ ε (ω) H m 1 1 m 1 2 eﬀ h = − − − . (7) 2 · ε (ω)ϕ εn(ω) εn(ω) eﬀ 2 − 1 Materials 2020, 13, 5639 12 of 15
For the series/parallel layer model (Figure9e), in which the near-surface layers are completely ﬁlled with ferroelectric and the central one is half ﬁlled, the penetration depth can be estimated as: εn (ϕ ) + εnϕ εn (ϕ ) + εn + εn ϕ + ε εn (ϕ + ) + εn εn ϕ H m 1 1 2 m 1 1 2 eﬀ 2 m 1 2 3 1 h = − − − . (8) 2 · 2ε ϕ εn εn eﬀ 2 − 1 On the basis of the considered Equations (1)–(8), the degree of ﬁlling of the porous glass matrix by BST were estimated, depending on the type of matrix and the treatment modes of the sample. The obtained parameters are shown in Table2. The spread in the values of 2 h/H is determined by the diﬀerent models used.
Table 2. Parameters of the NaFeSi/BST and LiFeSi/BST samples.
ε Sample Annealing Concentration of Pores, cm3/g eﬀ 2h/H (9.7 GHz) No 0.041 58 0.84 ... 0.94 LiFeSi/BST Yes 0.041 110 0.92 ... 0.98 No 0.033 40 0.82 ... 0.93 NaFeSi/BST Yes 0.033 55 0.91 ... 0.97
The results show the importance of annealing, which apparently improves the degree of impregnation of the porous system with the ferroelectric ﬁller.
4. Conclusions Glass-ceramic structures based on porous NaFeSi and LiFeSi glasses and barium-strontium titanate incorporated in the porous space were formed and studied using XRD, SEM, and porometry methods. The identiﬁcation of iron oxide in the glasses investigated was facilitated by Mössbauer spectroscopy. Electrical characteristics such as permittivity and losses of as-prepared and annealed in oxygen medium samples were also investigated in microwaves. The results of the studies conducted allow us to draw the following conclusions.
1. The method of obtaining porous glasses due to ion exchange between KFS glass and LiNO3 and NaNO3 melts allowed us to control a wide range of pore sizes and made it possible to form glass porous structures with pores of the required size. The ion exchange treatment between the cations of potassium-containing glass and NaNO3 and LiNO3 melts leads to the formation of porous structures with signiﬁcantly diﬀerent pore size distributions, which aﬀects the eﬃciency of the barium-strontium titanate insertion in a porous space and, consequently, the electrical characteristics of the structures. 2. XRD data indicate the presence of crystalline iron oxide, both in the initial glass and in the porous glass after ion exchange. The ion exchange procedure leads to a change in the phase composition and crystal structure of iron oxide. The ion exchange in the NaNO3 melt leads to a decrease in the content of the crystalline phase of iron oxide in the NaFeSi glass. On the contrary, the presence of rather intense reﬂexes of iron oxide in LiFeSi porous glass indicates a redistribution of the crystalline phases of iron oxide as a result of ion exchange. The charge state of iron in porous glass, and, consequently, the type of iron oxide—γ-Fe2O3 was determinated by Mössbauer spectroscopy. 3. Based on the porometric data and the results of electron microscopy, it can be assumed that the glass subjected to ion exchange in the LiNO3 melt shows a more developed porous structure, which has a positive eﬀect on the eﬃciency of introducing barium-strontium titanate into it. The impregnation of porous glasses with BST sol leads to uniform pore ﬁlling and the formation of a rather uniform surface without signiﬁcant cavities. Materials 2020, 13, 5639 13 of 15
4. Based on porous silicate glasses obtained by ion exchange, glass-ceramic materials containing a solid solution of barium-strontium titanate with a dielectric constant of more than 100 at microwaves were synthesized for the ﬁrst time. The resulting glass-ceramic structures were characterized by dielectric permittivity and losses, depending on the method of obtaining porous glass and high-temperature processing in an oxygen environment. An increase in the intensity of BST peak (111), an increase in permittivity, and a decrease in losses of glass-ceramic samples after annealing in oxygen conﬁrm the presence of crystalline BST in the pore space of NaFeSi and LiFeSi glasses. 5. Annealing of glass-ceramic structures in an oxygen environment has a positive eﬀect on their electrical characteristics. NaFeSi/BST glass-ceramic structures demonstrate a slight increase in the permittivity and a decrease in losses from 0.025 until 0.01 after the high-temperature treatment in oxygen. LiFeSi/BST structures look more preferable: the permittivity increases from 60 to 100, while the losses reduce by more than three times, from 0.05 to 0.02 as a result of annealing.
Author Contributions: Conceptualization, A.T., N.T. and N.M.; formal analysis, Z.T., N.M., A.G. and A.D.; funding acquisition, A.T.; investigation, A.T., N.T., Z.T., O.S., S.S., A.D., E.S. and I.M.; methodology, N.T. and S.S.; resources, Z.T., O.S. and S.S.; software, N.M.; supervision, A.T.; visualization, Z.T., O.S., A.G. and E.S.; writing—original draft, A.T., N.T. and N.M.; writing—review and editing, N.M. and A.G. All authors have read and agreed to the published version of the manuscript. Funding: This work was partially supported by the Russian Foundation for Basic Research under the project No 19-07-00600 A. Conﬂicts of Interest: The authors declare no conﬂict of interest.
1. Borderon, C.; Ginestar, S.; Gundel, H.W.; Haskou, A.; Nadaud, K.; Renoud, R.; Sharaiha, A. Design and Development of a tunable ferroelectric microwave surface mounted device. IEEE Trans. Ultrason. Ferroelectr. Freq. Contr. 2020, 67, 1733–1737. [CrossRef][PubMed] 2. Gupta, R.; Ranaa, L.; Sharmad, A.; Freundorfer, A.P.; Sayer, M.; Tomar, M.; Gupta, V. High frequency coplanar microwave resonator using ferroelectric thin ﬁlm for wireless communication applications. Mater. Today Proc. 2018, 5, 15395–15398. [CrossRef] 3. Romanofsky, R.R.; Toonen, R.C. Past, present and future of ferroelectric and multiferroic thin ﬁlms for array antennas. Multidimens. Syst. Signal Process. 2018, 29, 475–487. [CrossRef] 4. Nguyen, Q.M.; Anthony, T.K.; Zaghloul, A.I. Free-Space-Impedance-Matched composite dielectric metamaterial with high refractive index. IEEE Antennas Wirel. Propag. Lett. 2019, 18, 2751–2755. [CrossRef] 5. Wang, Q.; Li, S.; Oh, J.A.S.; Wu, T. Electrical impedance matching based on piezoelectric ceramics for energy harvesting application. Mater. Technol. 2020, 35, 650–655. [CrossRef] 6. Gowdhaman, P.; Annamalai, V.; Thakur, O.P. Piezo, ferro and dielectric properties of ceramic-polymer composites of 0-3 connectivity. Ferroelectrics 2016, 493, 120–129. [CrossRef] 7. Zhou, W.; Fan, J.; Xin, Z.; You, G. Micro-Structure modelling and electrical properties analysis of PZT matrix ferroelectric composites. Materials 2020, 13, 448. [CrossRef]
8. He, Y.; Peng, Y.; Xu, Y. The anomalous increase in tunability in Ba0.55Sr0.45TiO3-MgO-Mg2SiO4 composite ceramics. J. Am. Ceram. 2019, 102, 2706–2717. [CrossRef] 9. Nenasheva, E.A.; Kartenko, N.F.; Gaidamaka, I.M.; Redozubov, S.S.; Kozyrev, A.B.; Kanareykin, A.D. Low permittivity ferroelectric composite ceramics for tunable applications. Ferroelectrics 2017, 506, 174–183. [CrossRef] 10. Koroleva, E.Y.; Burdin, D.Y.; Kumzerov, Y.A.; Sysoeva, A.A.; Filimonov, A.V.; Vakhrushev, S.B. Dielectric
properties of magnetic-ferroelectric CoO–NaNO2–porous glass nanocomposite. Phys. Solid State 2017, 59, 2036–2044. [CrossRef] 11. Rysiakiewicz-Pasek, E.; Antropova, T.; Polyakova, I.; Pshenko, O.; Ci˙zman,A. New Insight into phase transitions of porous glass-based ferroelectric nanocomposites. Materials 2020, 13, 3698. [CrossRef][PubMed] Materials 2020, 13, 5639 14 of 15
12. Belysheva, D.N.; Sinel’shchikova, O.Y.; Tyurnina, N.G.; Tyurnina, Z.G.; Sviridov, S.I.; Tumarkin, A.V.; Zlygostov, M.V.; Ugolkov, V.L. Glycine–Nitrate synthesis of solid solutions of barium–strontium metatitanate. Phys. Solid State 2019, 61, 2371–2375. [CrossRef] 13. Tumarkin, A.V.; Al’myashev, V.I.; Razumov, S.V.; Gaidukov, M.M.; Gagarin, A.G.; Altynnikov, A.G.; Kozyrev, A.B. Structural properties of barium strontium titanate ﬁlms grown under diﬀerent technological conditions. Phys. Solid State 2015, 57, 553–557. [CrossRef] 14. Wu, J.-M.; Huang, H.-L. Microwave properties of zinc, barium and lead borosilicate glasses. J. Non-Cryst. Solids 1999, 260, 116–124. [CrossRef] 15. Letz, M. Microwave Materials and Applications; Sebastian, M.T., Jantunen, H., Ubic, R., Eds.; Wiley: New York, NY, USA, 2017; Volume 1, p. 345. 16. Kreisberg, V.A.; Antropova, T.V.; Kalinina, S.V. Eﬀect of the composition and conditions of the synthesis of porous glass on their micro- and mesoporous structures. Glass Phys Chem. 2014, 40, 501–512. [CrossRef] 17. Jones, J.R.; Ahir, S.; Hench, L.L. Large-Scale production of 3D bioactive glass macroporous scaﬀolds for tissue engineering. J. Sol-Gel Sci. Technol. 2004, 29, 179–188. [CrossRef] 18. Yatskovskaya, O.V.; Baklanova, O.N.; Gulyaeva, T.I.; Drozdov, V.A.; Gorbunov, V.A. The eﬀect of polyethylene glycol molecular weight on characteristics of the porous structure of silica materials. Prot. Met. Phys. Chem. Surf. 2013, 49, 216–221. [CrossRef] 19. Tallia, F.; Gallo, M.; Pontiroli, L.; Baino, F.; Fiorilli, S.; Onida, B.; Anselmetti, G.C.; Manca, A.; Vitale-Brovarone, C. Zirconia-containing radiopaque mesoporous bioactive glasses. Mater. Lett. 2014, 130, 281–284. [CrossRef] 20. Sviridov, S.I.; Tyrnina, Z.G.; Tyrnina, N.G.; Kryuchkova, L.Y.; Vlasenko, N.S. Ion-exchange formation of alkali silicate glass with a porous structure. Glass Phys. Chem. 2017, 43, 28–33. [CrossRef] 21. Sviridov, S.I.; Eliseeva, N.P. Interaction of glasses with nitrate melts in the systems containing Na+,K+, and Ba2+. Glass Phys. Chem. 1999, 25, 163–171. 22. Costa, F.; Borgese, M.; Degiorgi, M.; Monorchio, A. Electromagnetic characterization of materials by using Transmission/Reﬂection (T/R) devices. Electronics 2017, 6, 95. [CrossRef] 23. Tyurnina, Z.G.; Tyurnina, N.G.; Sviridov, S.I.; Vlasenko, N.S. Ion-Exchange Formation of Magnetic Iron-Containing Glass with a Porous Structure. Glass Phys. Chem. 2020, 46, 305–311. [CrossRef] 24. Siegrist, T. Crystallographica—A software toolkit for crystallography. J. Appl. Crystallogr. 1997, 30, 418–419. [CrossRef] 25. Lebedeva, S.M.; Bykov, V.N. Valent and structural state of iron ions in basalt glasses of diﬀerent crystallinity according to the data of Mössbauer spectroscopy. Geochem. Int. 2008, 46, 511–516. [CrossRef]
26. Ryu, S.S.; Lee, S.K.; Yoon, D.H. Synthesis of ﬁne Ca-doped BaTiO3 powders by solid-state reaction method—Part I: Mechanical activation of starting materials. J. Electroceramics 2007, 18, 243–250. [CrossRef] 27. Roy, A.C.; Mohanta, D. Structural and ferroelectric properties of solid-state derived carbonate-free barium
titanate (BaTiO3) nanoscale particles. Scr. Mater. 2009, 61, 891–894. [CrossRef] 28. Altynnikov, A.G.; Gagarin, A.G.; Gaidukov, M.M.; Tumarkin, A.V.; Petrov, P.K.; Alford, N.; Kozyrev, A.B.
Suppression of slow capacitance relaxation phenomenon in Pt/Ba0.3Sr0.7TiO3/Pt thin ﬁlm ferroelectric structures by annealing in oxygen atmosphere. Appl. Phys. Lett. 2014, 104, 042903. [CrossRef] 29. Tumarkin, A.; Gagarin, A.; Altynnikov, A.; Gaidukov, M.; Odinets, A.; Razumov, S.; Kozyrev, A. Eﬀect of
annealing in oxygen atmosphere on structure and microwave properties of multilayered tunable (Ba,Sr)TiO3 capacitors. Thin Solid Film. 2015, 593, 189–192. [CrossRef] 30. Chen, L.; Xiong, X.M.; Meng, H.; Lv, P.; Zhang, J.X. Migration and redistribution of oxygen vacancy in barium titanate ceramics. Appl. Phys. Lett. 2006, 89, 071916. [CrossRef] 31. Perry, N.H.; Kim, J.J.; Tuller, H.L. Oxygen surface exchange kinetics measurement by simultaneous optical
transmission relaxation and impedance spectroscopy: Sr(Ti, Fe)O3-x thin ﬁlm case study. Sci. Technol. Adv. Mater. 2018, 19, 130–141. [CrossRef] 32. Ascienzo, D.; Kurt, O.; Greenbaum, S.; Bayer, T.J.; Maier, R.A.; Randall, C.A.; Ren, Y. Formation of structural
defects and strain in electrodegraded Fe-doped SrTiO3 crystals due to oxygen vacancy migration. J. Am. Ceram. Soc. 2018, 101, 2545–2561. [CrossRef] 33. Rai, H.M.; Singh, P.; Saxena, S.K.; Mishra, V.; Warshi, M.K.; Kumar, R.; Rajput, P.; Sagdeo, A.; Choudhuri, I.;
Patha, B.; et al. Room-temperature magneto-dielectric eﬀect in LaGa0.7Fe0.3O3+γ; origin and impact of excess oxygen. Inorg. Chem. 2017, 56, 3809–3819. [CrossRef][PubMed] Materials 2020, 13, 5639 15 of 15
34. Fomin, A.A.; Fomina, M.A.; Rodionov, I.V.; Koshuro, V.A.; Poshivalova, E.Y.; Shchelkunov, A.Y.; Skaptsov, A.A.; Zakharevich, A.M.; Atkin, V.S. Superhard oxide coatings formed on titanium treated by high-frequency currents. Tech. Phys. Lett. 2015, 41, 909–911. [CrossRef] 35. Adilov, S.R.; Afanaciev, V.P.; Kashkul, I.N.; Kumekov, S.E.; Mukhin, N.V.; Terukov, E.I. Studying the composition and structure of ﬁlms obtained by thermal oxidation of copper. Glass Phys. Chem. 2017, 43, 272–275. [CrossRef] 36. Mukhin, N.; Afanasjev, V.; Sokolova, I.; Chigirev, D.; Kastro, R.; Rudaja, L.; Lebedeva, G.; Oseev, A.; Tumarkin, A. Heat-Resistant Ferroelectric-Polymer Nanocomposite with High Dielectric Constant. Materials 2018, 11, 1439. [CrossRef][PubMed] 37. Liu, G.; Chen, Y.; Gong, M.; Liu, X.; Cui, Z.-K.; Pei, Q.; Gu, J.; Huang, C.; Zhuang, Q. Enhanced dielectric performance of PDMS-based three-phase percolative nanocomposite ﬁlms incorporating a high dielectric constant ceramic and conductive multi-walled carbon nanotubes. J. Mater. Chem. C 2018, 6, 10829–10837. [CrossRef] 38. Barrow, D.A.; Petroﬀ, T.E.; Tandon, R.P.; Sayer, M. Characterization of thick lead zirconate titanate ﬁlms fabricated using a new sol gel based process. J. Appl. Phys. 1997, 81, 876–881. [CrossRef] 39. Yamada, T.; Ueda, T.; Kitayama, T. Piezoelectricity of a high-content lead zirconate titanate/polymer composite. J. Appl. Phys. 1982, 53, 4328–4332. [CrossRef] 40. Yoon, D.-H.; Zhang, J.; Lee, B.I. Dielectric constant and mixing model of BaTiO3 composite thick ﬁlms. Mater. Res. Bull. 2003, 38, 765–772. [CrossRef] 41. Tang, Z.; Scriven, L.E.; Davis, H.T. A three-component model of the electrical double layer. J. Chem. Phys. 1992, 97, 494–503. [CrossRef] 42. Wang, Q.; Tian, D.; Xiong, G.; Zhou, Z. A simpliﬁed model for the dielectric function of three-component composite materials. Phys. A Stat. Mech. Appl. 2000, 275, 256–261. [CrossRef] 43. Staskov,N.I.; Sotskaya, L.I. Three-Component Model of an Eﬀective Medium for Determining the Composition of Layers on Silicon Wafers. J. Appl. Spectrosc. 2017, 84, 764–769. [CrossRef] 44. Landau, L.D.; Lifshitz, E.M.; Pitaevskii, L.P.; Sykes, J.B.; Kearsley, M.J. Statistical Physics. Part I, 3rd ed.; Lifshitz, E.M., Pitaevskii, L.P., Eds.; Elsevier/Butterworth Heinemann: Amsterdam, The Netherlands; Boston, MA, USA, 1980; ISBN 9780750633727. 45. Ben Abdallah, N.; Degond, P.; Deluzet, F.; Latocha, V.; Talaalout, R.; Vignal, M.H. Diﬀusion Limits of Kinetic Models. In Hyperbolic Problems: Theory, Numerics, Applications; Hou, T.Y., Tadmor, E., Eds.; Springer: Berlin/Heidelberg, Germany, 2003; pp. 3–17, ISBN 978-3-642-62929-7.
Publisher’s Note: MDPI stays neutral with regard to jurisdictional claims in published maps and institutional aﬃliations.
© 2020 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (http://creativecommons.org/licenses/by/4.0/).